| ||Format||Pages||Price|| |
|2||$42.00||  ADD TO CART|
|Hardcopy (shipping and handling)||2||$42.00||  ADD TO CART|
Significance and Use
3.1 Unless there is a proper match between the expansions of the glaze and the body, all glazed whitewares may contain residual stresses from the firing that bonded the glaze to the body. In addition, whitewares are increasingly subjected to thermal stresses in service. Hence, an important use criterion for a glazed whiteware is adequate resistance to repeated abrupt thermal changes. In most cases, the result of inadequate resistance to thermal shock is the appearance of a craze pattern in the glaze. This craze pattern is visible by inspection with oblique lighting and application of a suitable ink or dye.
3.2 This test method is applicable to vitreous whitewares that have negligible crazing as a result of moisture expansion. For nonvitreous and semivitreous bodies, refer to Test Method .
1.1 This test method covers the determination of the resistance to crazing of fired, glazed, ceramic whitewares when stresses residual after glost firing may cause a tendency to craze, such stresses being induced by factors other than moisture expansion.
1.2 This test is not intended to induce moisture expansion, which fact should be kept in mind if the materials to be evaluated may exhibit moisture expansion.
Note 1: Test Method covers a method for determining resistance to crazing induced by moisture expansion. Its use is generally confined to testing nonvitreous and semivitreous ceramic whitewares because these products may be subject to such expansion. For whitewares with negligible moisture expansion (such as vitreous and impervious ware), the thermal shock method described herein is generally to be preferred.
1.3 The values stated in inch-pound units are to be regarded as the standard. The values in parentheses are for information only.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use. For a specific hazard statement, see Warning in .
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
C424 Test Method for Crazing Resistance of Fired Glazed Whitewares by Autoclave Treatment
ICS Number Code 81.060.20 (Ceramic products)
|Link to Active (This link will always route to the current Active version of the standard.)|
ASTM C554-93(2016), Standard Test Method for Crazing Resistance of Fired Glazed Ceramic Whitewares by a Thermal Shock Method, ASTM International, West Conshohocken, PA, 2016, www.astm.orgBack to Top